HAL Id: tel-02865536
https://tel.archives-ouvertes.fr/tel-02865536Submitted on 11 Jun 2020
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Faraday effect and using linearly polarized high order
To cite this version:
Carla Alves. Studying ultrafast magnetization dynamics through Faraday effect and using linearly polarized high order harmonics. Theoretical and/or physical chemistry. Sorbonne Université, 2018. English. �NNT : 2018SORUS328�. �tel-02865536�
École doctorale 388
Laboratoire Chimie Physique – Matière et Rayonnement (LCPMR) Laboratoire d’Optique Appliquée (LOA)
Studying ultrafast magnetization dynamics
through Faraday effect
and using linearly polarized high order harmonics
Par Carla Alves
Thèse de doctorat de Chimie Physique et Chimie Analytique
Dirigée par Jan Lüning
Présentée et soutenue publiquement le 14/12/2018 Devant un jury composé de :
Mme. Catherine Gourdon Directrice de Recherche Sorbonne Université (Président du jury) Mme. Annie Klisnick Directrice de Recherche Université Paris-Saclay (Rapporteur) M. Jan Vogel Directeur de Recherche Institut Néel (Rapporteur) M. Pascal Salières Directeur de Recherche CEA (Examinateur) M. Jan Lüning Professeur Sorbonne Université (Directeur de thèse) M. Guillaume Lambert Ingénieur de Recherche LOA (Invité)
“O que dá o verdadeiro sentido ao encontro é a busca, e é preciso andar muito para se alcançar o que está perto.”
List of Abbreviations ix
1 Fundamentals of ultrafast magnetism 5
1.1 Brief summary of the history of magnetism . . . 5
1.2 Magneto-optical effects . . . 8
1.2.1 Magneto-optical Faraday effect . . . 9
1.2.2 Magneto-optical Kerr effect . . . 11
1.2.3 Magnetic circular dichroism . . . 12
1.2.4 Resonant magnetic small-angle scattering . . . 13
1.3 Ultrafast magnetization dynamics . . . 14
1.3.1 Laser-induced demagnetization dynamics: historical review . . . 16
1.3.2 Models based on the Landau-Lifshitz equation . . . 17
1.3.3 Three temperature model . . . 19
1.3.4 Microscopic models for ultrafast demagnetization . . . 20
126.96.36.199 Elliott-Yafet Spin-flip events . . . 21
188.8.131.52 Spin super-diffusive transport . . . 22
1.4 Why X-rays for studying ultrafast magnetization dynamics? . . . 23
1.4.1 Typical experimental configuration . . . 25
1.4.2 EUV and X-ray sources around the world . . . 25
2 High order harmonic generation in gases 29 2.1 A suitable table-top source for ultrafast demagnetization measurements 29 2.2 Theory of the harmonics . . . 30
184.108.40.206 Three-step model: the semiclassical approach . . . 31
220.127.116.11 Lewenstein’s model: the quantum approach . . . 33
2.2.2 Phase matching . . . 34
2.2.3 Characteristics of the harmonics . . . 37
18.104.22.168 Spectral properties . . . 37
22.214.171.124 Description of the harmonics polarization state . . . 40
126.96.36.199.1 General concepts of polarized light . . . 40
188.8.131.52.2 Vector description of the light: Stokes-Mueller formalism . . . 43
184.108.40.206.3 Elliptically polarized high-order harmonics . . 45
2.3 Fundamental apparatus for HHG at LOA . . . 48
2.3.1 Laser system and laboratory environment . . . 48
2.3.2 IR optical system dedicated to HHG . . . 49
2.3.3 HHG systems . . . 51
2.3.4 Application section . . . 53
2.4 Potential optimization of our HHG source for magnetism studies . . . . 55
3 Towards ultrafast magnetization dynamics: Faraday effect using HHG 57 3.1 Introduction . . . 57
3.2 Static Faraday effect . . . 59
3.2.1 Theoretical relation between Faraday quantities and magnetization 59 3.2.2 Principle of the measurement . . . 62
3.2.3 Sample details . . . 64
3.2.4 Experimental apparatus . . . 65
3.2.5 Experimental results . . . 68
220.127.116.11 CoDy sample absorption . . . 68
18.104.22.168 Measurement of the Faraday effect through the harmon-ics footprint . . . 69
22.214.171.124 Measurement of the Faraday effect through the harmon-ics spectra . . . 71
126.96.36.199.1 CoDy alloy . . . 72
188.8.131.52.2 Co/Pt multilayer . . . 74
3.3.1 Pump-probe setup . . . 76
3.3.2 Time-resolved results . . . 78
184.108.40.206 Reference harmonic signal . . . 78
220.127.116.11 CoDy alloy . . . 79
18.104.22.168 Co/Pt multilayer . . . 82
Conclusions and Outlook 87
A Polarimetry of a low and even-order harmonic: 4ω 91
List of Abbreviations
3TM 3 Temperature Model BPM Bit-Patterned Media CCD Charge-Coupled Device EUV Extreme Ultra-Violet FEL Free-Electron Laser
GMR Giant Magneto-Resistance
HAMR Heat-Assisted Magnetic Recording HHG High Harmonic Generation
LCL Left- Circular Light
LCPMR Laboratoire de Chimie Physique - Matière et Rayonnement LLG Landau Lifshitz Bloch
LLG Landau Lifshitz Gilbert
L-MOKE Longitudinal Magneto-Optical Kerr Effect LOA Laboratoire d’Optique Appliquée
MCD Magnetic Circular Dichroism
MOKE Magneto-Optical Kerr Effect M3TM Microscopic 3 Temperature Model P-MOKE Polar Magneto-Optical Kerr Effect RCL Right- Circular Light
SAS Small-angle Scattering SFA Strong Field Approximation
T-MOKE Transverse Magneto-Optical Kerr Effect TMR Tunneling Magneto-Resistance
XFEL X-ray Free-Electron Laser
IntroductionThe quest for faster and smaller storage technology is one of the main interest of to-day’s society. The performance of these devices strongly depends on how fast the mag-netic properties of materials can be manipulated. And the information storage capacity depends on how small the magnetic materials can be reduced. Therefore, an advance-ment of this subject matter is as much in the interest of the industry as of the scientific community, regarding the wealth of the related discoveries. In this context, Beaurepaire et al.  made a great discovery in 1996 that opened an entirely new field of research. An ultrafast loss of the magnetization (<1ps) of a nickel film was observed after excita-tion of the magnetic layer by an intense femtosecond IR laser pulse. This observaexcita-tion was very surprising at the time, leading to the beginning of the laser-induced magne-tization dynamics research field. By applying an external magnetic field to a magnetic material, all the spins will be aligned leading to a macroscopic magnetization. A dy-namic response is induced when the direction of the magnetic field is suddenly turned. The magnetization must follow this external field giving rise to a reorientation of the spins. The process occurs within a few hundred femtoseconds after the magnetic sam-ple being perturbed by a femtosecond laser pulse. The electrons in the material quickly absorb part of the laser energy, creating a thermal disorder among their spins that re-sults in a lower magnetization. The mechanism behind this ultrafast loss is actively debated and no clear microscopic explanation of the experimentally observed effects in magnetic materials was accepted so far.
To follow such fast dynamics of magnetic materials for later technological applica-tions, two conditions are required for the laser source. First, short pulses are demanded to explore the dynamics on the femtosecond time scale. Second, the light source must cover the extreme ultraviolet or soft x-ray ranges to probe nanoscale magnetic materi-als. Both conditions are satisfied by the synchrotron femto-slicing and the FEL/XFEL
sources. The main drawback of these large-scale sources is the limited user accessibil-ity due to the small number of operational facilities worldwide. More accessible light sources in the extreme ultraviolet and soft X-rays ranges are based on the generation of high-order harmonics. The harmonic generation process is a nonlinear optical re-sponse of individual atoms in a gas while interacting with a laser beam. It offers an elegant approach to achieve table-top sources of coherent light with an ultra short flash of light, typically a few femtoseconds. For a long time, none of the available tools were fast enough to solve atomic and molecular dynamics. Consequently, harmonic sources have become an important key in many areas of investigation, including magnetism, making possible the study of ultrafast magnetization dynamics with high temporal res-olution and jitter free.
Magnetization phenomena is evaluated through magneto-optical effects, which de-scribe the interaction of magnetism with light. Therefore, high-order harmonic sources are commonly used in two different approaches regarding the polarization of the light, whether it is required elliptically or linearly polarized. Elliptically polarized light al-lows studies based on the magnetic circular dichroism , , which describes the dif-ferent response of a magnetized material to left and right-handed elliptically polarized light. Likewise, studies of magneto-optical effects using linearly polarized harmonics are performed, including the transverse magneto-optical Kerr effect – and mag-netic diffusion  techniques. While the transverse magneto-optical Kerr effect is exe-cuted in a reflection geometry retrieving information only about the material’s surface phenomena, the magnetic diffusion drawback, in a transmission geometry, lies on the difficulty of producing magnetic domains in the majority of the materials. The obser-vation of the magnetic circular dichroism in time-resolved experiments requires a very high degree of elliptically polarized harmonics with efficient fluence, which requires deeper investigations of the available techniques. Hence, for the first time we propose here to study the ultrafast magnetization dynamics through the Faraday effect, which goes beyond all those difficulties by using simply generated linearly polarized har-monics. The transmission geometry allows to probe all the layers of the material and no magnetic domains are required. Our approach is based on the resonant Faraday effect on the M absorption edge of transition metals, particularly between 40 and 70 eV for cobalt-based materials.
Thesis organization 3
This thesis reports the investigation of ultrafast magnetization dynamics in cobalt through the magneto-optical Faraday effect. Linearly polarized high-order harmonics are generated in noble gases in the extreme ultraviolet range to cover the entire M ab-sorption edge of cobalt. To accomplish this work, the following objectives were defined: • Assembly of the linearly polarized harmonic source for both static and
• Measurement of the static magneto-optical Faraday effect in cobalt based materi-als,
• Measurement of the evolution of the magnetization dynamics of cobalt based ma-terials through the Faraday effect,
• Accomplishment of the experiments using different thicknesses of cobalt based materials.
Chapter 1 includes the general scientific background behind this recent research field, the laser-induced ultrafast magnetization. The most relevant related theory and concepts for our experimental investigation are also reported.
The high-order harmonic source used to probe the magnetization dynamics of cobalt based materials is detailed in Chapter 2. In particular, the most important highlights of the theory behind the phenomenon as well as the experimental approach used in our work are presented. This chapter also focus on the importance of the high-order harmonic source for ultrafast magnetization dynamics studies. Additionally, the de-scription of the harmonics polarization state is presented along with some techniques used to obtain elliptically polarized light. This is related with my first experimental results performed at the beginning of my PhD, which are detailed in Appendix A.
The Chapter 3 refers to the experimental work that culminates the discussed points in the two previous chapters in an experimental realization. The experimental setup is explained in detail along with the principle of the measurement and the samples de-tails. The static and time resolved measurements are reported around the magnetically dichroic M absorption edge in CoDy and Co/Pt samples.
Fundamentals of ultrafast magnetismToday’s technology is intrinsically dependent on the phenomenon of magnetism. Ultrafast magnetization dynamics is a recent research topic which covers several pro-cesses occurring on a wide range of timescales. This chapter presents the general sci-entific background behind the laser-induced magnetization dynamics research field, as well as the relevant theory and concepts for the experimental investigation reported in this work.
Brief summary of the history of magnetism
Magnetism is an interesting phenomenon which plays an important role in the de-velopment of the civilization from the very beginning up to nowadays. Although its history dates back to earlier than 600 B.C., it was only in the twentieth century that scientists have begun to understand it and develop technologies based on this under-standing. In the northen Greece, in a city called Magnesia, a shepherd found a material with the ability to attract other pieces of the same material and iron. This material was a mineral magnetite called lodestone, which consists of iron oxide. The ancient Greeks called it a magnet because of the name of the city. Scientifically, William Gilbert (1540-1603) was the first to investigate the phenomenon of magnetism, discovering that Earth is itself a weak magnet. Early theoretical investigations into the nature of Earth’s magnetism were carried out by the german Carl Friedrich Gauss (1777-1855). Charles Coulomb (1736-1806) established the inverse square law of force, which states that the attractive force between two magnetized objects is directly proportional to the prod-uct of their individual fields and inversely proportional to the square of the distance
between them. Hans Christian Oersted (1777-1851) first suggested a link between elec-tricity and magnetism. Experiments showing the interaction between the effects of magnetic and electric fields were then conducted by Ampere (1775-1836) and Faraday (1791-1869). Also in the nineteenth century, Maxwell (1831-1879) provided the the-oretical foundation to the physics of electromagnetism. A full understanding of the magnetic effects on an atomic scale came in the late 1920’s with the advent of quantum mechanics by one of the founding fathers, Heisenberg (1901-1976) . From here new materials with wide applications in modern technology were created.
We can store information collected in a lifetime into a hard drive thanks to mag-netism. The discovery of the giant magneto-resistance (GMR) by Albert Fert and Peter Grünberg in 1988, is an important milestone in the history of magnetism. GMR refers to the large changes in electrical resistance observed in thin magnetic films and multi-layers depending on whether the magnetization of adjacent ferromagnetic multi-layers are in a parallel or an antiparallel alignment. The resistance can thus be manipulated by an externally applied magnetic field. This effect is widely used in hard-drive storage tech-nologies which have created a $50 billion industry. It is a great discovery which also marked the birth of spintronics, a new type of electronics where both the charge and the spin of electrons play a fundamental role. For example, the so-called spin polarized current, a current where the carriers have their spins oriented in the same direction, is created based on the GMR effect and used for many spintronics applications. A similar effect to the GMR is the tunneling magnetoresistance (TMR), whose effect relies on the possibility for electrons to tunnel between two magnetic layers –. The effect is being used in read heads to read/write in the computer hard discs. Areal density is defined as the number of bits in one inch square of hard-drive media. Conventional magnetic storage devices are limited to densities of 400 Gbits/in2 (i.e. one bit/40 × 40 nm2) and reading/writing times of 2 ns. Nowadays, the investigation focus on the quest for the smaller and the faster to understand the limits in the speed of the magne-tization dynamics and in the information storage capacity.
The heat-assisted magnetic recording (HAMR)  as well as the bit-patterned me-dia (BPM)  are promising for faster and higher capacity hard-drives in the future (figure 1.1). The HAMR uses a small amount of laser heating to increase the tempera-ture of recording spot (bit) to be able to switch the magnetization of the harder magnetic materials used to increase the bits density. Here, it is important to clearly understand
1.1. Brief summary of the history of magnetism 7
FIGURE1.1: Future hard-drive technologies. A schematic representation of the working principle of a) HAMR (from ), and b) conventional gran-ular media (blue arrow) and BPM (pink arrow) (from ).
the magneto-optical effects (MO) to be able to control the interaction between a laser pulse and a magnetic material. The BPM lies on the idea of using very small and well-organized grains, or bits, to make reading and writing processes much more efficient. Combining BPM and HAMR may lead to an areal density of 300 Tbits/in2, two or-ders of magnitude larger than the current commercial hard drives . Therefore, light sources in the extreme ultraviolet or soft x-ray range to probe magnetic nanostructures, and with short pulses to explore the dynamics on the femtosecond time scale, are im-portant for the development of future technologies.
This last magnetism research trend is not only on the interest of the industry and technology development: scientists are interested in the fundamental physics of mag-netic materials and the related dynamics at ultrafast time scales. In this context, the first observation of laser-induced ultrafast demagnetization in 1996  led to the develop-ment of a new field of research: ultrafast magnetization dynamics. After two decades of
increasing attention and research, the explanation behind the fundamental microscopic processes of the laser-induced magnetization dynamics is not well understood. In the rest of the chapter, this field is discussed, from the proposed theoretical hypothesis to the future applications, providing a bridge to the experimental results reported in this thesis.
Magneto-optical effects refer to interaction between light and a magnetized medium. These effects provide experimental support to the electromagnetic theory of light, as well as to both classical and quantum theory of matter. Using the MO effects, the mag-netic properties of the materials can be studied, and the magnetization manipulated and probed with light. Michael Faraday performed the first successful MO experi-ments in 1845 . He discovered that the polarization of a linearly polarized beam is rotated upon transmission through a material which is placed in a magnetic field parallel to the propagation direction of the light (figure 1.2 a)). In 1877, John Kerr ob-served the same effect in reflection , called the magneto-optical Kerr effect (MOKE) (figure 1.2 b)). Both effects arise from similar microscopic origins and can be explained
FIGURE1.2: Schematic representation of two MO effects configurations. a) Faraday, and b) MOKE effects.
using the same formalism. By definition, linearly polarized light can be decomposed in the sum of two circularly polarized waves, left- and right-circular polarized (LCL and RCL, respectively), with equal amplitude. The magnetization of the medium leads to the propagation of these two waves with (1) different velocities, and (2) experiencing different absorption rates. From (1) the polarization axis of the incident light will rotate
1.2. Magneto-optical effects 9 and from (2) the beam will change its polarization from linear to elliptical. Other im-portant MO effects are the magnetic circular dichroism (MCD) and the magnetic small-angle scattering (SAS). The MCD describes the differential absorption of left and right circularly polarized light, induced in a magnetized sample. In the SAS technique, the incident linearly polarized light is focused in a material with a magnetic domain struc-ture giving rise to magnetic scattering. In all the referred MO effects, a dependence of the complex refractive index with the magnetization is present. Nevertheless, in the next paragraphs, this dependence is only shown for the case of the Faraday effect.
Magneto-optical Faraday effect
The Faraday effect is schematically represented in figure 1.3 for an out-of-plane magnetized sample. As already mentioned, linearly polarized light can be decomposed into the sum of left- and right-circular polarized light. Consequently, each of the
com-z x y B B θF ƐF
FIGURE 1.3: Faraday effect illustration (adapted from ). The
polar-ization axis of the incident linearly polarized light (red line) changes upon transmission through a magnetized sample. θF and εFcorresponds to the
Faraday rotation and ellipticity, respectively.
ponents will experience a different refractive index as it propagates through a magnetic material. The complex refractive indices n±for these two circularly polarized waves describe the propagation of the radiation through the sample, where±refer to left- and
right-circular of the photon helicity relatively to the wave vector (~k) of the light,
n± =1− (δ0±∆δ) +i(β0±∆β). (1.1)
And in this particular case, where the sample’s surface is perpendicular to the prop-agation of the light (see figure 1.3), the magnetization of the sample (M) is parallel to~ ~k. In equation 1.1, ∆δ and ∆β are the intrinsic material’s magnetic-optical quantities, describing the Faraday rotation and ellipticity, respectively (θF and εF in figure 1.3). ∆δ
corresponds to the dephasing of the radiation, while∆β describes the absorption. For magnetized ferromagnetic materials, both are nonzero. In fact, if one of the circular waves travels faster than the other through the material, constituting a dephasing, it will also rotate faster generating the rotation of the light’s polarization axis . And the difference in absorption of the two circularly polarized waves changes the polariza-tion of the light from linear to elliptical.
Mathematically, the light transmitted through the sample propagating along the z axis is described as follows for the left- and right-circularly polarized waves ,
~E±(~r, t) = √1
where ω the frequency of the light. Both the phases and the amplitudes of the two circularly polarized waves have become unequal after passing through the sample. The ratio of the two electric field vectors for a sample with thickness d at normal incidence is then given by
From the Fresnel equation for the magnetic refractive indices of the material , θF
and εF can be related to n±by the equation
e2iθF =eiωd(n+−n−)/c. (1.4)
Since θF and εF are small compared to the nonmagnetic response, equation 1.4 can be
expanded to first order in the small quantities, which gives
θF+i tan εF ≈ ωd
1.2. Magneto-optical effects 11 The two Faraday polarization effects can thus be decomposed into two parts,
θF = ωd
2c <(n+−n−), (1.6)
tan εF = ωd
2c =(n+−n−). (1.7)
∆δ and ∆β can be obtained using the equation 1.1 in the above ones,
θF = −ωd
c ∆δ, (1.8)
tan εF = ωd
c ∆β. (1.9)
If the incoming light is not normal, but oblique (d =d0/ cos θt) at an incident angle θi , , θF = − Ephotd0 ¯hc tan θt∆δ, (1.10) tan εF = Ephotd0 ¯hc tan θt∆β. (1.11)
where Ephot is the photon energy, d0is the thickness of the foil and θt is the angle of
re-fraction. For x-ray light at the 2p edges, tan θt ≈tan θi. Thus,∆δ and ∆β can be directly
obtained from the experiment with small error. Although the first order approximation is valid in the soft-X-ray range, a more exact expression which relates both θF and εF to
the optical constants is required .
Magneto-optical Kerr effect
One can distinguish three main MOKE configurations which are represented in fig-ure 1.4. The plane xy is the plane of incidence. When magnetization M is in the plane~
FIGURE1.4: Different geometries for MOKE experiments (adapted from ). A schematic of the polarization state of the light is also represented before and after the light reflection on the sample.
of incidence and perpendicular to the sample surface, it corresponds to the polar geom-etry (P-MOKE). In longitudinal geomgeom-etry (L-MOKE), M is parallel to both the sample~ surface and plane of incidence. Lastly, in the transversal configuration (T-MOKE) con-figuration, theM remains parallel to the sample surface but perpendicular to the plane~ of incidence.
In the P-MOKE and the L-MOKE a polarization analysis is required to have infor-mation on the magnetization. On the contrary, in the T-MOKE there is no change in the polarization state since the magnetization is perpendicular to the plane of incidence. Here, the reflectivity of p-polarized light will give information on the amplitude and the direction of the magnetization .
Magnetic circular dichroism
Dichroism is defined as the property of some materials of absorbing light to different extents depending on the polarization form of the incident beam. Circular dichroism refers to the different absorption rates of the material for right- and left-handed circu-larly polarized light. When the effect is induced in a sample by a magnetic field parallel to the direction of light propagation, we refer to the magnetic circular dichroism (figure 1.5 a)). If the incident light is in the x-ray range, we refer to the XMCD. The effect is
FIGURE1.5: Principle of magnetic circular dichroism measurement. a) Schematic representation of the MCD, where the incident light (RCL or LCL polarized) is parallel to the sample’s magnetization (adapted from ). The transmitted light has different absorption coefficients depending on the helicity of the circularly polarized light, µ(−)and µ(+)for RCL and LCL, respectively. b) Absorption spectra measured at the L-edge of Fe for LCL and RCL helicities (from ).
1.2. Magneto-optical effects 13 related with the magnetism induced change in the absorption spectra, close to an ab-sorption edge of the material. The abab-sorption spectra measured at the material’s edge depends on the helicity of the circularly polarized light, as represented in figure 1.5 b) for LCL and RCL polarizations. The dichroism signal is then given by the difference between the two spectra corresponding to right- and left-handed circularly polarized light, which is described by the asymmetry of the absorption as follows,
The observation of the XMCD signal strongly depends on the orientation of the sam-ple’s magnetization, which is maximized when it is parallel or antiparallel to the po-larization axis of the incident light. XMCD has become a unique and widely used tool in magnetic spectroscopy allowing element specificity, which enables the characteriza-tion of different components in complex systems. In addicharacteriza-tion, quantitative informacharacteriza-tion about the orbital angular momentum and spin components of the magnetization can also be provided by the XMCD measurement. By increasing the thickness of the mag-netic material, the contrast level is improved. However, the drawback lies on the light transmission through the sample, which is exponentially reduced by the material thick-ness.
Resonant magnetic small-angle scattering
In SAS techniques, the radiation is elastically scattered by a sample and the result-ing pattern gives information on the size, shape, local magnetic moments, magnetic structure and phase transitions of the sample.
In some materials, it is possible to obtain a structure of magnetic domains having opposite magnetization directions at nanometer size by applying a specific demagneti-zation procedure . This structure acts as a grating that scatter light into a plus and minus first diffraction orders, as represented in figure 1.6 a). The scattered intensity in the first-order peaks is known to be proportional to the square of the magnetiza-tion magnitude within each magnetic domain, M2. We can then measure the dynamics of the magnetization by following the intensity of the scattering peaks (figure 1.6 b)). The scattering pattern can be observed with linearly polarized light since the light can
FIGURE 1.6: Magnetic small-angle scattering technique. a) Schematic representation of the technique where the structure of the sample acts as a grating that diffracts the light into two symmetric diffraction orders and, b) resonant magnetic scattering pattern of a domain structure at the cobalt M2,3absorption edge (from ).
be decomposed in the sum of right and left circularly polarized field of equal inten-sity. Many studies have been performed with the SAS technique using free-electron laser (FEL)  and high order harmonic generation (HHG) ,  sources. The main drawback of this technique lies on the limited type of materials in which magnetic do-mains are possible to obtain.
Ultrafast magnetization dynamics
Magnetization dynamics describes the evolution of the magnetization of a mate-rial, whose related processes occurs in a large range of timescales (figure 1.7). In the millisecond to second range, the thermal activated magnetization processes, such as viscous regime, domain nucleation and domain growth take place. From picosecond to nanosecond timescale, precessional and magnetic vortex dynamics as well as magnon generation and propagation and domain wall motion are observed. An easy way of
1.3. Ultrafast magnetization dynamics 15 inducing a dynamic response in a magnetic material is by applying an external mag-netic field. If the field is strong enough, all the spins tend to align in a ferromagmag-netic medium giving rise to a macroscopic magnetization. If the magnetic field direction is suddenly turned, the magnetization has to follow this external field. A reorientation of the spins occurs by a coherent damped precession of the spins around the external field as described by the Landau-Lifshitz-Gilbert equation , . The frequency of the precession is normally in the GHz range, corresponding to a period of a few hundreds of ps, and the reorientation process can take several nanoseconds. At the femtosecond regime, ultrafast demagnetization processes occur, related with the exchange interac-tion between spins. In specific, the ultrafast demagnetizainterac-tion process takes place within a few hundred fs after the magnetic sample being perturbed by a fs laser pulse. The electrons in the material quickly absorb part of the laser energy, creating a thermal dis-order among their spins that results in a lower magnetization. This process is several orders of magnitude faster than the timescales involved in precessional dynamics. Typ-ical demagnetization curves are shown in figure 1.8. It shows the timescale on which the demagnetization is quenched.
1.0 0.5 0 -500 0 500 1000 Magnetiz ati on (norm ali zed) Time delay (fs)
FIGURE1.8: Typical ultrafast demagnetization curves with different
de-magnetization degrees.After a femtosecond laser perturbation, a thermal disorder among the spins of the electrons in the material occurs, resulting in a lower magnetization.
The laser-induced ultrafast demagnetization research topic has high potential in technological applications, particularly magnetic storage technology. The process can
be useful for writing information in magnetic media in a very fast way. Therefore, two conditions are required for the light source:
1. short pulses to explore the dynamics on the femtosecond time scale, 2. extreme ultraviolet or soft x-ray range to probe magnetic nanostructures.
But these studies are still in the fundamental research stage, with no clear microscopic explanation for the experimentally observed effects in magnetic materials. In the next subsections, a brief overview of this phenomenon is presented.
Laser-induced demagnetization dynamics: historical reviewFirst experiments in laser excitation of ferromagnetic materials were conducted by Vaterlaus et al. , . The authors estimated that spin-lattice relaxation in Gd takes place within ∼100±80 ps. In other words, spin-orbit interactions cause electrons to lose their spin-angular momentum in the lattice, and as a result, the spin polarization of the electrons disappears. These experimental results along with theoretical predictions led to the conclusion that demagnetization upon laser heating follows from spin-lattice relaxation at a typical timescales between 0.1 and 1 ns.
In 1996, Beaurepaire et al.  observed the demagnetization dynamics of a Ni film via MOKE pumped, for the first time, with a very short pulse (60 fs). Surprisingly, the magnetization of Ni achieved its minimum value, almost 50% less than the satu-ration value, in less than 1 ps instead of the expected demagnetization time of some tens of ps (figure 1.9). This observation was soon confirmed by other groups ,  and the community has come to a full consensus about a typical demagnetization time within 100-300 fs. After the first observation of ultrafast demagnetization, a number of new investigations emerged. Laser-induced launching of magnetization precession and spin waves in canted ferromagnetic thin films was demonstrated . The loss of magnetization was directly detected by emission of terahertz radiation . Later, laser-induced magnetization dynamics in coupled multilayers was studied –.
Several hypothesis have been debated to explain the phenomenon of laser-induced ultrafast demagnetization from a microscopic point of view –. The main is-sue relies on understanding how angular momentum can be redistributed among elec-trons, spins and the lattice on such a short time scale. Indeed, magnetization is an-gular momentum and anan-gular momentum has to be conserved within the system. In
1.3. Ultrafast magnetization dynamics 17
FIGURE1.9: Beaurepaire et al. experimental observation of ultrafast de-magnetization in a Ni thin film (from ). The normalized remanence, proportional to the magnetization, drops in roughly 50% within the first ps, after fs optical excitation.
the following subsections, some models explaining ultrafast demagnetization are dis-cussed, starting with two phenomenological models, one based on the Landau-Lifshitz equation and the popular three temperature model. These two models describe the ex-perimental observations without taking explicitly into account the transfer of angular momentum. Afterwards, microscopic models explicitly considering the transfer of an-gular momentum for the underlying origin of ultrafast demagnetization are described.
Models based on the Landau-Lifshitz equation
The precessional motion of a magnetic moment is described by the Landau-Lifshitz equation ,
dt =γm~ × ~He, (1.13)
where γ is the gyromagnetic ratio and~Heis an effective magnetic field containing many
material dependent contributions, namely the external applied field, the anisotropy field and the demagnetization field.
In 1955, this equation was improved for the case of damping of a magnetic moment without magnitude change, the Landau-Lifshitz-Gilbert (LLG) equation ,
d~m dt =γ~m× ~He+ α |~m|m~ × d~m dt , (1.14)
with α being a dimensionless phenomenological Gilbert damping constant. But this is valid only at low temperature and for no change of the magnetic moment magnitude. Therefore, one can use the Landau-Lifshitz-Bloch (LLB) equation , which is valid up to and beyond the Curie temperature TC, to describe changes in the magnetization
vector norm. d~m dt =γm~ × ~He−γλk ~ m(~m· ~He) m2 +γλ⊥ ~ m× (~m× ~He) m2 , (1.15)
where λk and λ⊥are the dimensionless longitudinal and transversal damping
parame-ters . The three contributing terms of the LLB equation is schematically represented in figure 1.10.
M-m ( m · He) m × (m × He) m × He
FIGURE 1.10: Illustration of the Landau-Lifshitz-Bloch equation (adapted from ). The three terms of the equation 1.15 are represented. The red force corresponds to the first term, which makes the magnetic mo-ment precessing around He. The second term matches the green force,
which is the source of demagnetization by longitudinal damping. Finally, the blue force corresponds to the third term, which applies a transversal damping to align the magnetic moment along He without changing its
The LLG and LLB equations successfully describes some ultrafast demagnetization dynamics experiments , ,  but no assumptions are made about the micro-scopic mechanisms behind the damping parameters.
1.3. Ultrafast magnetization dynamics 19
Three temperature model
Beaurepaire et al.  introduced a phenomenological three temperature model (3TM), based on the two-temperature model that assumes that electrons and the lattice are dif-ferent coupled heat reservoirs by defining the temperature of the electrons and phonons. In the three temperature model, the spin-degree of freedom was added as a third reser-voir, describing then the interaction between the electrons (e), spins (s) and lattice (l), as sketched in figure 1.11 a). The temporal evolution of the system’s temperature is described by the following coupled differential equations :
Ce(Te)dTe dt = −Gel(Te−Tl) −Ges(Te−Ts) +P(t), (1.16) Cs(Ts)dTs dt = −Ges(Ts−Te) −Gsl(Ts−Tl), (1.17) Cl(Tl) dTl dt = −Gel(Tl−Te) −Gsl(Tl−Ts), (1.18)
where P(t) represent the initial excitation from the laser, C the heat capacities and T the temperature of the three systems. Gel, Ges and Gsl are the coupling constants between
electrons and lattice, electrons and spins, and spins and lattice, respectively. Once de-termined, G gives information about the strength of a particular link but does not deter-mine the nature of the interaction. The laser excitation with a femtosecond laser pulse
FIGURE 1.11: Three temperature model. a) Schematic diagram with the
respective interaction time constants between the reservoirs (adapted from ). b) Experimental observation of spin (Ts), lattice (Tl), and electron (Te)
is initially almost instantaneously absorbed by the electrons. The heat is then redis-tributed among the three systems through the previous equations, following by spin and then lattice. The temperature evolution between different reservoirs after the laser excitation is schematically shown in figure 1.11 b).
Nevertheless, the three temperature model is not sufficient to completely under-stand the microscopic mechanisms involved in laser-induced demagnetization. Once more, the angular momentum conservation should be considered in the magnetic sys-tem, which explains what happen with the spins during full demagnetization process . This problem is discussed in the following subsection.
Microscopic models for ultrafast demagnetization
Despite more than two decades of research, the microscopic quantum interpreta-tion for the ultrafast demagnetizainterpreta-tion is still under debate by the scientific commu-nity. Figure 1.12 shows a schematic timeline of the possible ultrafast photon-electron-spin-lattice interactions after an excitation by an ultrafast laser . To clarify the
phe-FIGURE 1.12: Schematic timeline of ultrafast photon-electron-spin-lattice interactions after an ultrafast laser excitation (adapted from ). A laser excitation on the electron system trigger various scattering pro-cesses between electrons and phonons. First, the excited electron system thermalizes by electron-electron scattering and the material starts to de-magnetize because of spin-flip scattering and superdiffusive spin currents events during this thermalization process. Then, electron-phonon scatter-ing processes transfer energy from the excited electrons to the lattice, and thermal equilibrium is typically reached on picosecond timescales. Lastly, the system riches the equilibrium by thermal diffusion on nanosecond timescales.
1.3. Ultrafast magnetization dynamics 21 nomenon of ultrafast demagnetization, the importance of the contribution of each rep-resented interaction during the process has to be established, specially the understand-ing of the angular momentum dissipation in a femtosecond timescale.
In this subsection, I present the two most discussed microscopic models. The first one based on the Elliott-Yafet Spin-flip events and the second based on the mechanism of spin super-diffusive transport.
22.214.171.124 Elliott-Yafet Spin-flip events
To explain the ultrafast demagnetization dynamics, Koopmans et al.  proposed to consider electron-phonon scattering event of Elliott-Yafet type . Upon collision with a phonon, an electron has a probability as f to flip its spin. This model presupposes
FIGURE1.13: Schematic representation of the Elliott-Yafet spin-flip scat-tering. The electron changes its spin upon emission of a phonon, taking over angular momentum (from ).
that the angular momentum is directly transferred from the spin to the lattice. Later, in another investigation, Koopmans et al. proposed another model which combines the three temperature model with the Elliott-Yafet mechanism, the so-called the micro-scopic three temperature model (M3TM) . In this model, ab initio calculations of the Elliot Yafet spin flip probabilities were considered. The behavior of Cobalt and Nickel demagnetization were successfully reproduced with this model. In the meantime, Es-sert et al.  concluded that electron-phonon spin-flip scattering is not sufficient to explain the experimental results behind ultrafast demagnetization. Furthermore, the dynamical changes of the band structure are important but they are not included in the M3TM. These last results infer that the Elliott-Yafet spin flip scattering phenomena cannot explain alone the demagnetization rate experimentally observed.
126.96.36.199 Spin super-diffusive transport
In 2010, Battiato et al.  proposed another mechanism to explain the ultrafast de-magnetization behavior based on a spin dependent transport of hot electrons, called the spin super-diffusive transport. In this work, theoretical demagnetization curves of a Ni/Al bilayer and a Ni reference sample were compared to understand the differ-ent processes unleashed by laser excitation. The idea of the model is to verify if the electrons of the Al layer are excited by the effect of super-diffusive spin transport, as schematically represented in figure 1.14. It is shown that the spin majority electrons ("spin up") leave the excited region more promptly than the spin minority electrons ("spin down"), leading thus to femtosecond spin currents. The demagnetization of the excited region is an immediate consequence of the reduction of the number of spin majority electrons.
FIGURE1.14: Sketch of the super-diffusive phenomena created by a laser excitation. Majority and minority spin carriers show different mean free paths and also a cascade of electrons is generated after an inelastic scatter-ing (from ).
Other interesting investigations on utrafast spin dynamics were carried out by Rudolf et al.  using a Ni/Ru/Fe trilayer. The magnetization of the Ni and Fe layers can be either parallel or antiparallel (figure 1.15 a)). If the magnetization of Ni and Fe are par-allel, the Ni layer magnetization decreases while the Fe is enhanced by the demagneti-zation of Ni, as plotted in figure 1.15 b). When they are antiparallel, the magnetidemagneti-zation of both Ni and Fe layers decreases, as shown in figure 1.15 c). The results for these two systems on the femtosecond timescale infer the generation of super-diffusive spin current between Fe and Ni layers after optically induced demagnetization, which is in good agreement with the spin super-diffusive transport model. On the other hand, Schellekens et al.  revealed that spin transport is negligible in the demagnetization
1.4. Why X-rays for studying ultrafast magnetization dynamics? 23
FIGURE1.15: Layer- and time-resolved magnetization of Ni and Fe lay-ers (from ). a) Illustration of parallel and antiparallel magnetization alignment of the Ni and Fe layers, where the red and green circles are the majority spin alignment in the layers, and the large white arrow represents the flow of the spin current. b) and c) corresponds to the time-resolved magnetization of the Fe (red) and Ni (blue) layers for parallel and antipar-allel magnetization alignment, respectively.
process of ferromagnetic films on insulating substrates by comparing front-pump with back-pump measurements of a Ni/Al2O3 film. Therefore, the spin current is certainly
not the dominant effect in the demagnetization of ferromagnetic Ni films.
Why X-rays for studying ultrafast magnetization
The development of future technologies is based on the full understanding of the dynamics of nanoscale magnetic materials at ultrashort timescales. Therefore, light sources at short wavelengths with short pulses on the femtosecond timescale are desir-able to probe nanoscale magnetic structures. With visible light, ranging from 400 to 800 nm, optical microscopy can only detect objects down to approximately 200 nm in size, which is already larger than the bit size used in commercial hard drives. Consequently,
there is a quest for light sources on the extreme ultraviolet (EUV) and soft x-ray range to probe nanoscale magnetic materials. EUV light ranges from 30 to 250 eV, and soft x-rays range from 250 eV to several keV, which allows a spatial resolution below hun-dred nanometers allowing applications such as microscopy  and lithography . Here, the spatial resolution is small enough to study the hard drives structures up to an areal density of 10 Tbits/in2in EUV and 1000 Tbits/in2in soft x-rays, as schematically represented in figure 1.16.
Ultraviolet Extreme Ultraviolet Soft X-rays Hard X-rays
1Tbits/in² 10Tbits/in² 100Tbits/in² 1000Tbits/in²
10eV Infrared Microwaves Radar Ultraviolet Gamma rays Hard X-rays Co M-edge L-edgeCo 100nm 1000nm 1millimeter 1nm
FIGURE 1.16: Wavelength resolvable bit size and associated areal
stor-age density. EUV and soft x-ray range allow to study nanoscale magnetic structures with high resolution due to the their short wavelengths (black and gray for the wavelength and photon energy, respectively). The respec-tive areal densities for different wavelengths are also represented (red). Additionally, the Co M and L absorption edges are represented in green.
From the scientific point of view, many interesting absorption edges of magnetic materials and rare earths correspond to the EUV and soft x-ray regions. The interaction of magnetism with light is studied through MO effects, as detailed in subsection 1.2. Near the EUV and soft x-ray absorption edges, the MO effects are greatly enhanced which allows the observation of very small effects. Furthermore, the absorption edges are unique for each element which is very useful in magnetism based applications, such as probing magnetization in an element-specific manner. For example, ferromagnetic elements, e.g., iron, cobalt, and nickel, have absorption edges located in EUV and soft x-ray regions. M absorption edges, where core 3p electrons are excited to the valence 3d
1.4. Why X-rays for studying ultrafast magnetization dynamics? 25 levels, are located at the EUV region. The soft x-ray region corresponds to L absorption edges, where deeper core 2p electrons are excited to the same valence 3d levels. In this thesis, we focused on the study of the M-edge of cobalt materials.
Typical experimental configuration
The ideal experimental technique should combine sensitivity to the magnetization state with femtosecond time resolution. In addition, it should allow element selectivity, meaning distinguish different materials in an alloy or a multilayer system, and image with nanometer spatial resolution (for future technological applications).
Typical experiments employ the pump-and-probe method. A femtosecond laser pulse in the optical range (pump) first excites a magnetic system. Then, a delayed sec-ond pulse (probe) of eletromagnetic radiation resolves the ultrafast dynamics in the material. Repeating this procedure for several time delays, a reconstruction of the tem-poral evolution of the excitation taking place in the medium is possible. The duration of the probe pulse defines the temporal resolution. The spectrum of the probe should be chosen according to the material absorption edges one is interested to investigate, far-infrared, optical, ultraviolet, or x-ray spectral ranges. Further complete information can be obtained while measuring the same phenomenon for the four different ranges. In my work, a probe pulse on the EUV/soft x-ray range is required for the investigation of the M absorption edge of cobalt-based materials.
EUV and X-ray sources around the world
Femto-slicing at sychrontron , , X-ray free-electron laser (XFEL) facilities , , and table-top HHG sources , – are complementary techniques with unique advantages. All of them present the nanometer-wavelength and femtosecond-pulse-duration requirements for element-selective studies of ultrafast magnetization dynamics. Synchrotrons and XFELs can probe high energy absorption L-edges. HHG probes mainly absorption M-edges but with the advantage of simultaneously prob-ing the magnetic dynamics of multiple wavelengths and jitter free. In terms of output energy, femto-slicing and HHG sources are similar delivering up to 1 µJ, while FEL sources reach 100 µJ.
Traditional synchrotron radiation is generated by accelerating electrons bunches to relativistic speed and put them in a circular storage ring: when the path of the bunches is altered (acceleration) either by a bending magnet or an undulator, radiations are emit-ted covering the spectral range from infrared to hard x-ray. It presents a large photon flux and the pulse duration range from a few hundred picoseconds to nanoseconds. But in the slicing mode, the pulse duration goes down to∼100 fs , which is adapted to capture ultrafast magnetization dynamics. XFELs provide very bright short-pulsed light across the electromagnetic spectrum. The process uses a linear accelerator for ac-celerating a beam of electrons close to the speed of light. The electrons pass through a long periodic arrangement of permanent magnets, which creates a sigmoidal magnetic field. This magnetic field forces an oscillating trajectory of the electrons and, conse-quently the emission of an electromagnetic wave train . The main drawback of these large-scale light sources is the limited user accessibility because of the very small number of operational slicing beamlines and XFELs worldwide (figure 1.17).
More accessible light sources for extreme ultraviolet and soft x-rays are based on high-order harmonic generation. This table-top source was employed in the course of this thesis for studying magnetization dynamics of the M absorption edge of cobalt materials and it is described in detail in Chapter 2.
1.4. Why X-rays for studying ultrafast magnetization dynamics? 27
FIGURE 1.17: Large-scale light sources. a) XFEL (from ) and b) syn-chrotron (from ) facilities worldwise and in Europe, respectively.
High order harmonic generation in
gasesThe generation of high order harmonics occurs due to a highly nonlinear optical process when an intense laser, typically 1014−15 W/cm2, with some tens of fs pulse is focused in a gas. This is a non destructive and table-top source of spatially ,  and temporally coherent  and polarized light, ranging from the ultraviolet (260 -100 nm) to the soft X-ray region (-100 - 10 nm) , . HHG presents a wide range of applications, including nonlinear EUV optics , attosecond physics –, EUV spectroscopy  or ultrafast magnetism . This chapter presents the HHG, particu-larly the theoretical models, the general experimental approach and its importance for ultrasfast magnetization dynamics studies.
A suitable table-top source for ultrafast
Harmonic emission is a coherent nonlinear response of individual atoms, first ob-served in 1961 by Franken et al.  shortly after the demonstration of the first working laser by Maiman in 1960. The experiment consisted in focusing light from a pulsed ruby laser (at 694.3 nm wavelength,∼3 J pulse energy and 1 ms pulse duration) into a non isotropic crystalline quartz sample. As a result, the second harmonic of the fundamen-tal beam at 347.2 nm was generated with a very low efficiency conversion. This became the first experiment in the nonlinear optics field. In 1967, New et al. demonstrated the first third-harmonic generation in a gas .
High order harmonic generation was first observed by McPherson et al.  who successfully generated harmonic emission up to the 17thorder with a 248 nm radiation in neon gas. When it was first reported, the main research lied on understanding its physical phenomena –. It was then followed by the development of a coherent light source in the EUV region –. In the last 15 years, the main research topic was focused on attosecond science –. Basically, HHG is an elegant approach to achieve table-top sources of coherent light with the shortest flash of light, typically a few hundreds of attoseconds.
For a long time, no available tools were fast enough to resolve atomic and molecular dynamics, so HHG has become an important key in such investigation fields. However, the drawback of the HHG-based sources lies on the poor efficiency in their conversion of energy, 10−7 in neon , 10−5 in argon , and slightly below 10−4 in xenon, as well as the limitation to energies around a few hundred eV. But in order to time-resolve intra-nuclear dynamics it is necessary an advancement to shorter pulse duration and higher photon energies.
In addition, investigations of HHG polarization control have been performed, con-stituting an important tool in magnetic spectroscopy based techniques. HHG sources allow the investigation of ultrafast spin dynamics for up to a few femtoseconds jitter free temporal resolution. For example, it allows the reconstruction of the ultrafast laser-induced magnetic evolution. A new quantum control method  and spectroscopy method  in the EUV region are under development, which involve the active use of attosecond pulse trains.
Theory of the harmonics
In a traditional optics theory, the low applied electric field (E) of the light and the dielectric polarization (P) of a material is given by a linear relationship:
2.2. Theory of the harmonics 31 For stronger electric fields (up to 108 V/m), the nonlinear terms in the induced po-larization become important, which can be expressed by the Taylor series
The first term defines the linear susceptibility and the next ones the nonlinear suscep-tibilities, which are small compared to the first one. Typically, only laser light is suf-ficiently intense to modify the optical properties of a material system. Its response to an applied optical field depends in a nonlinear manner on the strength of the optical field. When a very strong laser field is applied, a very high order of the polarization is induced. HHG is an extreme nonlinear optical process which occurs in the strong field regime. A completely new perturbative understanding of nonlinear optics is then necessary to describe the high order harmonics processes. Several models have been proposed to explain the occurrence of high order harmonics generated by individual atoms. The models are based on the behavior of a single atom exposed to the electric field of the laser. Two main approaches will be here discussed: a semiclassical model and a quantum model.
188.8.131.52 Three-step model: the semiclassical approach
The most successful description is the three-step model from Corkum et al. . It is a semiclassical model since both quantum and classical approaches are used to de-scribe the electron behavior. From quantum mechanics, a quantum particle presents an undulatory structure, which defines the measurement of the probability of finding the particle within a certain location. Therefore, the quantum approach describes the electron as a superposition of waves or a electronic wave packet. Classically, the model is based on the application of Newton’s physics to study the movement of ionized elec-trons in the electric field of the linearly polarized driving laser. The three steps of the model are represented in figure 2.1. First, the gas interacts with the electric field of an intense laser beam, which lowers the potential barrier of the atoms of the gas (1). In every half optical cycle, an electron can be emitted by tunnel ionization and then accel-erated by the laser field in the continuum, gaining kinetic energy (2). When the laser field changes the sign, it is slowed down and then accelerated towards its parent atom. Finally, when the electron passes near the atom, it has a certain probability to recombine
on the ground state (3). When the electron recombines, a photon, with energy equal to the one gained by the acceleration in the field plus the ionization potential, is emitted in the form of a strong and coherent HHG photon in the EUV. These three steps are described in more details in the next paragraphs.
1. Tunneling ionization Ip ℎν = Ip+Up 3. Recombination and photoemission 2. Continuum propagation
FIGURE2.1: Three-step model of high-harmonic generation with linear
polarization in a gas (adapted from ). 1, Distortion of the Coulomb potential due to the electric field of the focused laser, inducing tunnel-ionization of an electron. 2, The electron wave packet is accelerated away from the atom. 3, Due to electric field reversal the electron wave packet is accelerated back and then recombines with the parent ion when the field is nearly zero, leading to the emission of extreme ultraviolet radiation.
One considers an isolated atom in the fundamental state. An electron in this con-dition is submitted to the Coulomb potential of the nucleus, V0 = −1/r. Adding a
linearly polarized electromagnetic field, E(t) = Excos(ω0t)ex, where ex and ω0
corre-sponds to the polarization axis and the angular frequency of the field, the new potential becomes:
V(x, t) =V0(x) +xE(t) (2.3)
This leads to the lowering of the potential barrier on one side. If the field is strong enough, part of the electronic wave packet can cross the potential barrier by tunneling effect. This probability depends on the height, thickness and the time during which this barrier is lowered. By further increasing the intensity of the electric field, the po-tential barrier is completely removed, releasing the electron. This extreme case is called ionization regime by barrier suppression , .
Continuum propagation, recombination and photoemission
After tunneling out of the atom, we assume that the electronic wave packet dy-namics is ruled only by the laser field, strong enough to neglect the long-range atomic
2.2. Theory of the harmonics 33 potential effects. We can then use the classical description of the electronic wave packet dynamics, where the Lorentz force is the only one acting on the electron:
m¨x = −eE0cos(ω0t) (2.4)
For the initial conditions, ti is the instant of the wave packet ionization, and one
as-sumes x(ti) = 0 and ˙x(ti) = 0, meaning the movement across the tunnel barrier is
neglected and all its kinetic energy is lost after crossing it. Integrating the equation 2.4:
˙x = − eE0 mω0[sin(ω0t) −sin(ω0ti )] (2.5) x = eE0 mω02[cos(ω0t) −cos(ω0ti)] + eE0 mω0 sin(ω0ti)(t−ti) (2.6)
The electron oscillates in the field in the direction ex and periodically returns to x = 0,
that is its parent atom, where it can recombine, emitting a EUV photon. The electron’s trajectory depends on the time of its emission into the continuum. A photon is emitted only when the electrons leaves the atom at every half cycle of the driving laser (maxi-mum and mini(maxi-mum of the laser field). The periodicity is then T/2, where T = 2π/ω0
is the period of the laser, corresponding to 2ω0in the frequency domain. The spectrum
of the emitted radiation is therefore a harmonic comb up to a cut-off energy (see equa-tion 2.13), described in detail in secequa-tion 2.2.3, separated by 2ω0. Moreover, since the
generation medium is centro-symmetric, only the odd harmonics are emitted.
The three-step model gives a simple picture of the HHG process, successfully ex-plaining the experimental observations, like the prediction of the cut-off region. How-ever, a quantitative description requires more advanced quantum mechanical calcula-tions, including a more realistic treatment of the atomic system. This is explained in further detail in the next section.
184.108.40.206 Lewenstein’s model: the quantum approach
In 1994, Lewenstein et al.  proposes a fully quantum model of the single atom emission of HHG, which takes into account the quantum effects not included in the semiclassical model. In the semi-classical model, a single electron is considered to ac-celerate along a certain trajectory, by the electric field of the laser, while in this quantum mechanical description, an ensemble of trajectories will contribute to the wave packet.
This approach is based on the Strong Field Approximation (SFA). Considering only one active electron submitted to the electric field~E(t), the Schrodinger equation is written:
i∂| ψ(~x, t)i ∂t = (− 1 2∇ 2+V(~x) − ~E· ~x) | ψ(~x, t)i (2.7)
Lewenstein et al. solved numerically the time dependent Schrödinger equation in a strong field with the following assumptions:
• The contribution to the wave packet of all bound states except the ground state can be neglected,
• There is no depletion of the ground state,
• In the continuum states, the electron can be treated as a free particle moving in the electric field with no effect of the atomic potential.
The electron, propagating in the laser field, recombines with the parent ion by a dipole transition. The SFA approach assumes the calculation of the harmonic dipole moment as the coherent sum of all the different quantum paths that contribute to the harmonic emission. In addition, this model shows the dependence of the conversion efficiency on the laser wavelength and pulse duration. Lasers with shorter wavelength as well as lasers with shorter pulse duration, generate harmonics more efficiently. From these approximations, also the cut-off law is predicted,
Emax =IpF(Ip/Up) +3.17Up, (2.8)
where Up and Ip are the ponderomotive and the atom ionization potentials,
respec-tively. The factor F(Ip/Up) is equal to 1.3 when Up Ip, and ∼ 1 when Ip increases.
This equation is in good agreement with both the semiclassical three step model and with experimental data.
An important property of HHG is its coherence, which arises because the phase of harmonic emission is locked to the laser phase. So, for example, if the laser has linear polarization, the harmonics will have linear polarization. But for a HHG conversion process to be efficient, it is crucial for the emission that all atoms are phase-matched
2.2. Theory of the harmonics 35 meaning that harmonics from different atoms have to be emitted with the same phase to allow for constructive interferences throughout the medium length (figure 2.2). In turn, the intensity of harmonic radiation will grow as square of the medium length. There is an additional phase shift between the fundamental laser field and the
gener-FIGURE2.2: Schematic representation of phase-matching (adapted from ).Two cases of generation are represented: non-phase-matched (∆k6= 0) and phase-matched (∆k=0).
ated harmonics field, produced when the ionized electron transfers an additional phase acquired during its movement in the electric field. This can affect the properties of the resulted beam, such as angular distribution  or coherence , giving rise to the phase mismatch between them, which restricts the quadratic growth of the harmonic intensity with the medium length. The phase matching effect on the high order har-monics generated in gas medium was first studied in . To maximize the emission, the wave vector mismatch, ∆k, must be minimized. For a given harmonic order q, in conventional nonlinear optics,∆k is equal to
where kq e kL are the wave vectors of the harmonic field and fundamental laser,
Lc = π/∆k, which describes the propagation distance between two locations of
har-monic emission that are exactly out of phase. Thus, within Lc the two fields,
funda-mental and harmonic, interfere constructively. Outside this limit, destructive interfer-ences between them occur, meaning that at the end of the coherence length, there is a π phase shift between the two fields that was generated at the beginning of the coherence length.
With regard to the macroscopic emission corresponding to the HHG, the equation 2.9 must be considered in the strong field regime to include the harmonic dipole phase gradient :
Minimization of the phase mismatch in HHG and optimization of its conversion effi-ciency has been studied extensively , –. There are four main contribu-tions that can result to phase shift between the incoming laser beam and the generated harmonics:
The Gouy phase shift∆kg contributes when a laser beam induces a geometrical phase
mismatch associated with the rapid variation of the Gouy phase at the Gaussian beam focus. This gradient depends on the spatial coordinates and always takes negative values. The minimum value is at the beam focus, equal to−q/zR, where zR = πω20/λ
is the Rayleigh length, with ω0the beam waist. ∆kaand∆kp are due to the atomic and
plasma dispersion, respectively, making different frequencies (fundamental laser and harmonics) travel with different velocities in the medium. Finally, the harmonic dipole phase gradient∆kd is the partial derivative of the phase gained by the electron in the
continuum, also leading to an atomic phase mismatch.
Furthermore, the medium where HHG are produced reabsorbs the radiation, espe-cially in the EUV region of the spectrum. This limits the medium length to 5-10 times the absorption length :
(2.12) where ρat is the atomic density and σabs(λ) is the absorption cross-section,
decreas-ing with the harmonic order. The optimal conversion for the generation conditions is L > 3Labs and Lc > 5Labs, where L is the medium length, as plotted in figure 2.3. In
2.2. Theory of the harmonics 37
FIGURE2.3: HHG photon emission as a function of the medium length in units of absorption length (from ).The dotted line refers to the no absorption case.
summary, the phase-matching terms are dependent on the setup parameters, the ge-ometry, and the generation medium. And a change of one parameter often influences many phase-matching terms. Consequently, the optimization of the HHG generation requires a persistent readjustment so that all the setup parameters match.
Characteristics of the harmonics
220.127.116.11 Spectral properties
The harmonic radiation is emitted in the form of a comb of the odd multiple fre-quencies of the fundamental frequency of the driving laser (ω). Contrary to a contin-uous exponential decrease typical for perturbative nonlinear processes, three different spectral regions can be defined in the emission spectrum of HHG (figure 2.4). In the perturbative region (3th −7th harmonic) the intensity of each harmonic order drops rapidly, then levels out in a plateau of successive harmonics with similar intensity until a sudden cut-off within a few harmonic orders. The cut-off law which defines the max-imum HHG photon energy generated from a single atom is determined by the sum of the atom ionization potential, Ip, and by the ponderomotive potencial, Up: